DOI 10.1007/s10948-013-2142-3 O R I G I N A L PA P E R
Effects of Excess or Deficiency of Oxygen Content
on the Electronic Structure of High-T
CupratesT. Jarlborg· A. Bianconi · B. Barbiellini ·
R.S. Markiewicz· A. Bansil
Received: 2 December 2012 / Accepted: 14 February 2013 / Published online: 15 March 2013 © Springer Science+Business Media New York 2013
Abstract Band structure calculations are presented for large supercells of Ba2CuO4 (BCO) with O-vacancies in planar or apical positions, and of superoxygenated La2CuO4 (LCO) with oxygen interstitials in the La2O2 layers. It is found that apical oxygen vacancies in BCO act as elec-tron dopants and makes the elecelec-tronic structure similar to that of hole doped LCO. Excess oxygen interstitials form-ing wires in the La2O2layers of LCO are shown to yield a much larger density-of-states at the Fermi energy than for the stoichiometric compound related with a segmentation of the Fermi surface. Antiferromagnetic (AFM) spin fluctua-tions are strengthened by O-vacancies in BCO as well as by oxygen interstitials in LCO, but are strongly suppressed in O-deficient LCO. Our results indicate the complexity of doping by O-vacancies, and by ordered defects that are a significant factor controlling the electronic properties of cuprates.
Keywords Cuprates· Electronic structure · Oxygen defects
T. Jarlborg ()
DPMC, University of Geneva, 24 Quai Ernest-Ansermet, 1211 Geneva 4, Switzerland
e-mail:Thomas.Jarlborg@unige.ch A. Bianconi
RICMASS, Rome International Center for Materials Science Superstripes, Via dei Sabelli 119A, 00185 Rome, Italy B. Barbiellini· R.S. Markiewicz · A. Bansil
Department of Physics, Northeastern University, Boston, MA 02115, USA
High-Tc cuprate superconductors in their normal state show many unusual properties such as pseudogaps, stripe-like charge/spin modulations with particular energy/doping dependencies, Fermi-surface (FS) “arcs” in the diagonal di-rection, ‘kinks’ and ‘waterfalls’ in the band dispersions, anomalous isotope effect, and phonon softening [1, 2]. It is generally believed that stripe-like modulations of the Cu-spin arrangements are important for doped cuprates. Band results for long ‘1-dimensional’ (1-D) supercells, calculated by the Linear Muffin-Tin Orbital (LMTO) method in the local density approximation (LDA), show large spin-phonon coupling (SPC) within the CuO planes [3,4]. The LMTO results have been used to parameterize the strength of potential modulations coming from phonon distortions and spin waves of different length . Phonon softening, dynamical stripes, correlation between ¯q and x, smearing of the non-diagonal part of the FS, and abrupt disappear-ance of spin fluctuations at a certain T∗, are all possible consequences of SPC within a rather conventional band pic-ture [5,6]. Weak ferromagnetism is a possibility at very high hole doping levels [7,8]. The focus has been for many years on the intrinsic electronic response of the CuO2plane following electronic doping pushing the chemical potential away from half filling. The details of the structure of spacer layers intercalated between the CuO2 planes and the role of dopants, atomic substitutions, defects or oxygen intersti-tials inserted there to convert the undoped antiferromagnetic CuO2plane into a superconductor has not been much con-sidered so far.
Recently there has been growing interest to control the superconducting Tc by changing the structure of the spacer layers. It is known that maximum superconducting Tcat op-timum doping increases from 20 to 130 K by manipulation
of the spacer layers structure  and the spatial distribu-tion of defects inserted there. For example the maximum superconducting Tc in La2CuO4 (LCO) achieved through La/Sr or La/Ba exchange is 35 K while with the maximum Tc in superoxygenated La2CuO4+δ can reach 45 K. Re-cently the ordering of oxygen interstitials has been shown to control the superconducting Tc [10,11]. High Tc’s have been reported for oxygen deficient Sr2CuO4−δ[12–14] and in other cuprates with ordered defects . Moreover the dopants and their self organization have been shown to con-trol the critical temperature in pnictides  and chalco-genides .
Here we present aspects of our results of band structure calculations on supercells of Ba2CuO4(BCO) or La2CuO4 (LCO) with various distributions of O-defects for the pur-pose of gaining insight into how the electronic structure and magnetic interactions are modified by the presence of such defects. For oxygen deficient structures it matters if the va-cancies are located within the CuO2planes or in apical posi-tions. In the latter case the vacancies act as electron dopants of the Cu-d band, so that BCO with a substantial apical-vacancy concentration would approach the band filling of hole doped LCO. Excess oxygen interstitials inserted in the rocksalt La2O2 layers of LCO occupy the oxygen intersti-tial positions as oxygen ions in fluorite Nd2O2spacer layer of Nd2CuO4.
We show here the breakdown of the common rigid band model for doped CuO2planes. Defects induce a band fold-ing and openfold-ing of partial gaps at specific points in the k-space and produce multiple mini-bands crossing the Fermi level as has been proposed . Moreover the ordered oxy-gen interstitials yield a much larger density-of-states at the Fermi energy than for the stoichiometric compound, favor-ing enhanced spin fluctuations.
A more complete discussion of these results will be un-dertaken elsewhere [19,20].
2 Method of Calculation
Ab-initio LDA-LMTO band calculations are carried out for supercells of R2CuO4±δ, with R= La or Ba (LCO or BCO). In the case of oxygen vacancies in LCO and BCO, the calcu-lations are based on supercells with a total of 112 sites . The supercell is obtained via a 2× 2 × 2 extension of the basic antiferromagnetic (AFM) cell, R32Cu16O64−nV, where nV is the number of O-vacancies in the cell. Different con-centrations δ= nV/16 of vacancies either in the planes (P) or in apical (A) positions are realized through a randomized (not clustered) distribution of vacancies in R2CuO4−δ.
For simulating ordered stripe-like interstitial oxygens, we first insert empty spheres in all interstitial positions at (12,0,12c) and (0,12,12c), and then occupy one or two of
these positions with additional oxygen interstitials. In total, this yields a supercell with 72 sites for a 4× 1 × 1 extension of the basic AFM cell along the diagonal[1, 1, 0]-direction, La16Cu8O32+N, where N is the number of additional oxy-gens. There are one or two adjacent rows of additional O in the supercells . The atomic spheres are reduced com-pared to the calculations for the 112-site supercell, but the results for defect free LCO are very similar in the two sets of calculations.
Spin-polarized calculations are made with applied mag-netic fields on selected Cu-sites in order to generate AFM order. Other details of our band calculation methods have been published elsewhere [19–21]. It should be noted that a rigid band picture  or its variants  have often been invoked in describing the doping evolution of the overdoped and optimally doped cuprates [24,25]. Our large supercell treatment here goes beyond the simple rigid band model or possible mean-field type approaches [26,27] to elucidate the local electronic and magnetic properties of the system.
3 Results for O-Deficient BCO and LCO
Unpolarized calculations show that apical or planar oxygen vacancies act very differently with respect to d-band filling and charge on Cu . Apical vacancies in BCO lead to a charge transfer toward Cu and an upward shift of EF rel-ative to the d-band, so that the band structure of BCO with many vacancies can approach that of hole doped LCO.1 Api-cal vacancies in LCO have a similar but weaker doping ef-fect, whereby LCO becomes electron doped. Vacancies in the planes of LCO lead to hole doping, while in BCO the ef-fect on doping is small. These results are interesting in view of recent reports of high Tc in oxygen deficient SCO , although possibility of some type of ordering has been im-plicated [13,15]. A question that arises naturally in this con-nection is whether the propensity for AFM fluctuations cor-relates with the effective doping level, since spin fluctuations are probably involved in the mechanism of superconducting pairing. Accordingly, in our calculations we mimic an AFM order by applying positive or negative magnetic fields on every second Cu. We have taken the AFM structure and the field amplitudes to be identical in all cases investigated in order to make direct comparisons between BCO and LCO with different types of defect.
Our main results are summarized in Table 1. For va-cancies in CuO planes of BCO there is, in addition to the weak hole doping within the Cu-d band, a tendency toward stronger AFM fluctuations. The enhancement is similar for
1Note that Ba and Sr have one less electron than La, which makes BCO
Table 1 Valence charge QCu(in electrons/per Cu), the change QCu
with respect to the undoped case, and the magnetic moment m (in μB
per Cu) as a function of the number (nV)of planar (P) or apical (A)
oxygen vacancies in BCO and LCO. A magnetic field of±2.5 mRy was applied to generate AFM order on Cu
nV BCO LCO QCu QCu ¯m QCu QCu ¯m 9 (P) 10.055 −0.010 0.024 10.332 −0.063 0.010 8 (P) 10.056 −0.009 0.022 – – – 5 (P) 10.057 −0.007 0.024 10.368 −0.026 0.025 1 (P) 10.062 −0.002 0.021 10.395 −0.000 0.073 0 10.064 0.000 0.020 10.394 0.000 0.069 1 (A) 10.071 0.007 0.021 10.420 0.026 0.069 5 (A) 10.107 0.043 0.028 10.450 0.056 0.024 8 (A) 10.145 0.081 0.038 – – – 9 (A) 10.163 0.099 0.035 10.456 0.062 0.022
vacancies on the apical positions, in spite of the clear elec-tron doping in this case. The evolution of AFM fluctuations for O-vacancies in LCO is very different. Undoped LCO has strong enhancement of AFM waves that leads to a stable AFM configuration and an insulator. Well converged LSDA calculations do not find this state, but it has been shown that LMTO calculations with off-center linearization energies of the Cu-d states lead to slight localization and stable AFM or-der . Both apical and planar vacancies quickly suppress the tendency for antiferromagnetism as seen in Table1. This agrees qualitatively with early calculations for a single O va-cancy in small unit cells of LCO .
Interestingly, we find that the electron doping effect in BCO with apical vacancies is strong, and one may ask if the properties of such crystals are similar to those of hole doped LCO. Our results indicate that it is not exactly so, since antiferromagnetism in BCO with the highest elec-tron doping is selec-tronger than in LCO where maximal hole doping is made via planar O-vacancies. In LCO, it seems that breaking the near neighbor order through apical or pla-nar O-vacancies will effectively quench AFM fluctuations, much like the effect of Sr doping. An example can be seen in Fig. 1, where the local moment on Cu is plotted as a function of the local Cu valence charge for configurations with nine O-vacancies. These results suggest that local or-der is probably an important factor for antiferromagnetism. The increasing strength of spin fluctuations with increasing number of apical vacancies provides a possible explanation for why oxygen deficient SRO can have a higher Tc than the traditional hole doped LCO. Doping is usually thought to be determined by the La vs. Sr/Ba substitution, but our results show that oxygen deficiency may have large effects on doping as well. For instance, electron doping usually car-ried out through La/Nd–Ce substitution is accompanied with a structural change of the apical O position, but our results
Fig. 1 Absolute value of the magnetic moment m as function of the
valence charge for each Cu-atom in BCO and LCO with nine apical or planar O-vacancies
show that apical O-vacancies in LCO could provide an al-ternate route for electron doping keeping the structure in-tact.
4 Results for Stripes of Oxygen Interstitials in the Spacer Layers
Rows of single or double interstitial O’s oriented along [1,1,0] make the DOS at EF larger than in undoped LCO by factors of 2.5 or 3, respectively, see Fig.2. The new O-p bands associated with the interstitials are found to lie a few eV below EF, but hybridization effects make the bands at
EF narrower. The interstitial oxygens and the neighboring atoms acquire most of the additional DOS. This increase in DOS comes about because the band at EF is broken up by the new periodicity with smaller dispersion between the re-sulting small gaps. A folding of the original almost circular LCO Fermi surface (FS) into the new Brillouin Zone (BZ), given by Γ –R–X3–M3, produces a FS similar to the one in Fig.3. The computed FS for the undoped supercell (N= 0) of LCO agrees even more with the model where circular FS in the original BZ has been downfolded into the BZ of the supercell. One difference is that the FS’s for the super-cells containing extra O are segmented with gaps between the branches. The three branches in Fig. 3 corresponds to different sections of the circular FS in the original BZ. Fur-thermore, the calculated band mass increases when one or two O atoms are added, and bands become gapped near the boundaries of the new BZ. A general upward displacement of the FS branch in the left part of Fig.3can be understood from an increased radius of the original FS. This represents
Fig. 2 The total DOS of the undoped La16Cu8O32near the Fermi level
is compared with the DOS of doped superoxygenated La2CuO4with
additional N= 1 and N = 2 oxygen interstitial in the supercell
Fig. 3 The calculated FS for La16Cu8O32+Nfor N= 2. This FS can be understood from a folding of the original circular FS into the Bril-louin Zone of the supercell (given by Γ –R–X3–M3), but the partial
gaps appears only for N > 0
hole doping, which is consistent with effective charges on Cu: Addition of each interstitial O in the cell removes about 0.04 electrons from each Cu.
The new periodicity sets up a potential modulation along the unit cell and as expected induces weak pseudogaps in the DOS near EF. It turns out that EF falls on a DOS peak above the gap energy, both for one and two extra oxygen atoms. Thus, the observation of ordering of oxygen intersti-tials [11,30] might be a promising way for creating potential modulations, pseudogaps and enhanced N (EF)for boost-ing superconductivity . Furthermore, FS segmentation and small gaps separating mini bands could provide favor-able conditions for Lifshitz transitions in connection with other mechanisms for enhanced Tc . Notably, the en-hanced N (EF)favors AFM fluctuations in general . The calculation of modulated AFM spin waves shows a moder-ate increase of the exchange enhancement when one or two O-interstitials are added, but the effect concerns mostly Cu sites far from the interstitials. The strong hybridization with the additional O-p electrons, which are not magnetically
ac-tive, is probably the cause of the limited effect on nearby Cu sites.
Our study shows that electronic properties of cuprates can be modified substantially by the presence of oxygen defects. In particular, vacancies among apical and planar oxygen sites lead to very different charge filling within the Cu-d band, and strong changes in the AFM couplings in the system. Moreover, AFM fluctuations in BCO and LCO behave quite differently as a function of doping. The effective doping de-pends not only on La/Ba substitutions, but also on the spe-cific nature of oxygen vacancies. For excess O, we follow the suggestions from experiments and assume that intersti-tial oxygens order into stripes. The new periodicity makes the DOS high at EF, which leads to some enhancement of AFM fluctuations. The FS branches remain fairly intact and identifiable for different doping, but mini-gaps are formed to make the FS segmented. Heavier band masses are evident as well as a slight hole doping for increasing O content. These changes are normally favorable to a higher Tc.
Acknowledgements This work is supported by the US Department of Energy contract number DE-FG02-07ER46352, and benefited from the allocation of supercomputer time at the NERSC and Northeastern University’s Advanced Scientific Computation Center (ASCC).
1. Damascelli, A., Shen, Z.-X., Hussain, Z.: Rev. Mod. Phys. 75, 473 (2003) and references therein
2. Armitage, N.P., Fournier, P., Greene, R.L.: Rev. Mod. Phys. 82, 2421 (2010)
3. Jarlborg, T.: Phys. Rev. B 64, 060507(R) (2001) 4. Jarlborg, T.: Phys. Rev. B 68, 172501 (2003) 5. Jarlborg, T.: Physica C 454, 5 (2007)
6. Jarlborg, T.: Phys. Rev. B 76, 140504(R) (2007)
7. Barbiellini, B., Jarlborg, T.: Phys. Rev. Lett. 101, 157002 (2008) 8. Sonier, J.E., Kaiser, C.V., Pacradouni, V., Sabok-Sayr, S.A.,
Cochrane, C., MacLaughlin, D.E., Komiya, S., Hussey, N.E.: Proc. Natl. Acad. Sci. USA 107, 17131 (2010)
9. Bianconi, A., Agrestini, S., Bianconi, G., Di Castro, D., Saini, N.L.: J. Alloys Compd. 317, 537 (2001)
10. Fratini, M., Poccia, N., Ricci, A., Campi, G., Burghammer, M., Aeppli, G., Bianconi, A.: Nature 466, 841 (2010)
11. Poccia, N., Fratini, M., Ricci, A., Campi, G., Barba, L., Vittorini-Orgeas, A., Bianconi, G., Aeppli, G., Bianconi, A.: Nat. Mater. 10, 733 (2011)
12. Liu, Q.Q., Yang, H., Qin, X.M., Yu, Y., Yang, L.X., Li, F.Y., Yu, R.C., Jin, C.Q.: Phys. Rev. B 74, 100506 (2006)
13. Gao, W.B., Liu, Q.Q., Yang, L.X., Yu, Y., Li, F.Y., Jin, C.Q., Uchida, S.: Phys. Rev. B 80, 094523 (2009)
14. Geballe, T.H., Marezio, M.: Physica C 469, 680 (2009)
15. Chmaissem, O., Grigoraviciute, I., Yamauchi, H., Karppinen, M., Marezio, M.: Phys. Rev. B 82, 104507 (2010)
16. de Montellano, G.S.O., de Leon, J.M., Saini, N.L., Bianconi, A.: J. Appl. Phys. 111, 112631 (2012)
17. Ricci, A., Poccia, N., Joseph, B., Arrighetti, G., Barba, L., Plaisier, J., Campi, G., Mizuguchi, Y., Takeya, H., Takano, Y., Saini, N.L., Bianconi, A.: Supercond. Sci. Technol. 24, 082002 (2011)
18. Perali, A., Bianconi, A., Lanzara, A., Saini, N.L.: Solid State Commun. 100, 181 (1996)
19. Jarlborg, T., Barbiellini, B., Markiewicz, R.S., Bansil, A.: Phys. Rev. B 86, 235111 (2012). doi:10.1103/PhysRevB.86.235111 20. Jarlborg, T., Bianconi, A.: Phys. Rev. B 87, 054514 (2013).
21. Jarlborg, T.: Appl. Phys. Lett. 94, 212503 (2009) 22. Bansil, A.: Z. Naturforsch. A 48, 165 (1993)
23. Lin, H., Sahrakorpi, S., Markiewicz, R.S., Bansil, A.: Phys. Rev. Lett. 96, 097001 (2006)
24. Sahrakorpi, S., Lindroos, M., Markiewicz, R.S., Bansil, A.: Phys. Rev. Lett. 95, 157601 (2005)
25. Bansil, A., Lindroos, M., Sahrakorpi, S., Markiewicz, R.S.: Phys. Rev. B 71, 012503 (2005)
26. Bansil, A., Rao, R.S., Mijnarends, P.E., Schwartz, L.: Phys. Rev. B 23, 3608 (1981)
27. Mijnarends, P.E., Bansil, A.: Phys. Rev. B 13, 2381 (1976) 28. Sterne, P.A., Wang, C.S.: Phys. Rev. B 37, 7472 (1988) 29. Jarlborg, T.: J. Phys. Condens. Matter 16, L173 (2004)
30. Poccia, N., Ricci, A., Campi, G., Fratini, M., Puri, A., Di Gioacchino, D., Marcelli, A., Reynolds, M., Burghammer, M., Saini, N., Aeppli, G., Bianconi, A.: Proc. Natl. Acad. Sci. USA
109, 15685 (2012)
31. Innocenti, D., Caprara, S., Poccia, N., Ricci, A., Valletta, A., Bian-coni, A.: Supercond. Sci. Technol. 24, 015012 (2011)